MSE_2610_HW_5

# MSE_2610_HW_5 - MSE 2610 Introduction to the Mechanical...

This preview shows pages 1–2. Sign up to view the full content.

MSE 2610 Introduction to the Mechanical Properties of Materials Fall 2008 Homework Assignment #5 1.) Hexagonal close-packed (HCP) zinc slips only by basal plane slip. A zinc single crystal is oriented so that the normal to its slip plane makes an angle of 60° with the tensile axis. The three slip directions have angles of 38°, 45°, and 84° with respect to the tensile axis, and the critical resolved shear stress (CRSS) is 2.3 MPa. The shear modulus G for the crystal is 42 GPa. a.) Determine the tensile stress at which plastic deformation commences. b.) The lattice parameters for zinc are a = 2.66 Å and c = 4.94 Å. What is the magnitude of the Burgers vector b ? c.) What is the critical force per unit length (of dislocation) required to move a straight dislocation in zinc? d.) What is the length of the shortest dislocation line segment that could act as a double-ended dislocation source ( i.e. , Frank-Read source), if the maximum shear stress acting on the dislocation segment is 5.2 MPa?

This preview has intentionally blurred sections. Sign up to view the full version.

View Full Document
This is the end of the preview. Sign up to access the rest of the document.

{[ snackBarMessage ]}

### Page1 / 2

MSE_2610_HW_5 - MSE 2610 Introduction to the Mechanical...

This preview shows document pages 1 - 2. Sign up to view the full document.

View Full Document
Ask a homework question - tutors are online